text: The most elaborately accurate, but totally destructive, precious metal assay is fire assay. (It may also be called by the critical cupellation step that separates precious metal from lead.) If performed on bullion to international standards, the method can be accurate on gold metal to 1 part in 10,000. If performed on ore materials using fusion followed by cupellation separation, detection may be in parts per billion. However, accuracy on ore material is typically limited to 3 to 5% of reported value. Although time-consuming, the method is the accepted standard applied for valuing gold ore as well as gold and silver bullion at major refineries and gold mining companies.
  In the case of fire assaying of gold and platinum ores, the lengthy time required to carry out an assay is generally offset by carrying out large numbers of assays simultaneously, and a typical laboratory will be equipped with several fusion and cupellation furnaces, each capable of taking multiple samples, so that several hundred analyses per day can be carried out. The principal advantage of fire assay is that large samples can be used, and these increase the accuracy in analyzing low-yield ores in the <1g/T range of concentration.
  Fusion: the process requires a self-generating reducing atmosphere, and so the crushed ore sample is mixed with fluxes and a carbon source (e.g. coal dust, ground charcoal, flour, etc.) mixed with powdered lead oxide (litharge) in a refractory crucible. In general, multiple crucibles will be placed inside an electric furnace fitted with silicon carbide heating elements, and heated to between 1,000 and 1,200 °C. The temperature required, and the type of flux used, are dependent on the composition of the rock in which the precious metals are concentrated, and in many laboratories an empirical approach based on long experience is used.
  A complex reaction takes place, whereby the carbon source reduces the lead oxide to lead, which alloys with the precious metals: at the same time, the fluxes combine with the crushed rock, reducing its melting point and forming a glassy slag. When fusion is complete, the sample is tipped into a mold (usually iron) where the slag floats to the top, and the lead, now alloyed with the precious metals, sinks to the bottom, forming a button. After solidification, the samples are knocked out, and the lead bullets recovered for cupellation, or for analysis by other means.
  Method details for various fire assay procedures vary, but concentration and separation chemistry typically comply with traditions set by Bugby or Shepard & Dietrich in the early 20th century. Method advancements since that time primarily automate material handling and final finish measurements (i.e., instrument finish rather than physical gold product weighing). Arguably, even these texts are largely an extension of traditions that were detailed in De re metallica by Agricola in 1556.
  Variation from skills taught in modern standard adaptations of fire assay methodology should be viewed with caution. The standard traditions have a long history of reliability; "special" new methods frequently associate with reduced assay accuracy and fraud.
  Cupellation: the lead bullets are placed in porous crucibles (cupels) of bone ash or magnesium oxide and heated in air to about 1,000 °C. This is usually carried out in a muffle furnace, containing a refractory muffle (usually nitride-bonded silicon carbide) heated externally by silicon carbide heating elements. A flow of air through the muffle assists oxidation of the lead, and carries the fumes for safe collection outside the furnace unit. The lead melts and oxidises to lead oxide, which in turn melts and is drawn into the pores of the cupel by capillary attraction. The precious metals remain in the base of the cupel as a prill which is sent for final analysis of precious metal content.
  In the bullion fire assay process, a sample from the article is wrapped in a lead foil with copper and silver. The wrapped sample, along with prepared control samples, heated at 1,650 °F (or 898.9 °C; temperature varies with exact method) in a cupel made of compressed bone ash or magnesium oxide powder. Base metals oxidize and absorb into the cupel. The product of this cupellation (doré) is flattened and treated in nitric acid to remove silver. Precision weighing of metal content of samples and process controls (proofs) at each process stage is the basis of the extreme method precision. European assayers follow bullion traditions based in hallmarking regulations. Reputable North American bullion assayers conform closely to [http://www.astm.org/Standards/E1335.htm ASTM method E1335-04e1]. Only bullion methods validated and traceable to accepted international standards obtain genuine accuracies of 1 part in 10,000.
  Cupellation alone can only remove a limited quantity of impurities from a sample. Fire assay, as applied to ores, concentrates, or less pure metals, adds a fusion or scorification step before cupellation.